ASTM C183 : Sampling and the Amount of Testing of Hydraulic Cement
Được đăng lên bởi
kien098
Số trang: 6 trang

Lượt xem: 787 lần

Lượt tải: 0 lần
Designation: C 183 – 97 Standard Practice for Sampling and the Amount of Testing of Hydraulic Cement1 This standard is issued under the fixed designation C 183; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (e) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense. 1. Scope 1.1 This practice covers procedures for sampling and for the amount of testing of hydraulic cement after it has been manufactured and is ready to be offered for sale. 1.2 The values stated in SI units are to be regarded as the standard. The inchpound units in parentheses are for information purposes only. 1.2.1 A ton as used in this practice is 907 kg (2000 lb). 1.2.2 Values in SI units shall be obtained by measurement in SI units or by appropriate conversion, using the Rules for Conversion and Rounding given in Standard IEEE/ASTM SI 10, of measurement made in other units. 1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. C 204 Test Method for Fineness of Hydraulic Cement by Air Permeability Apparatus2 C 227 Test Method for Potential Alkali Reactivity of CementAggregate Combinations (MortarBar Method)3 C 265 Test Method for Calcium Sulfate in Hydrated Portland Cement Mortar2 C 266 Test Method for Time of Setting of HydraulicCement Paste by Gillmore Needles2 C 451 Test Method for Early Stiffening of Hydraulic Cement (Paste Method)2 C 452 Test Method for Potential Expansion of Hydraulic Cement Mortars Exposed to Sulfate2 C 563 Test Method for Optimum S03 in Hydraulic Cement Using 24 h Compressive Strength2 C 595 Specification for Blended Hydraulic Cements2 C 845 Specification for Expansive Hydraulic Cement2 C 1012 Test Method for Length Change of HydraulicCement Mortars Exposed to a Sulfate Solution2 E 11 Specification for WireCloth Sieves for Testing Purposes4 IEEE/ASTM SI 10 Standard for Use of the International System of Units (SI): The Modern Metric System4 2.2 ACI Standard: 225.1R Guide to the Selection and Use of Hydraulic Cements5 2. Referenced Documents 2.1 ASTM Sta...
Designation: C 183 – 97
Standard Practice for
Sampling and the Amount of Testing of Hydraulic Cement
1
This standard is issued under the ﬁxed designation C 183; the number immediately following the designation indicates the year of
original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A
superscript epsilon (e) indicates an editorial change since the last revision or reapproval.
This standard has been approved for use by agencies of the Department of Defense.
1. Scope
1.1 This practice covers procedures for sampling and for the
amount of testing of hydraulic cement after it has been
manufactured and is ready to be offered for sale.
1.2 The values stated in SI units are to be regarded as the
standard. The inchpound units in parentheses are for informa
tion purposes only.
1.2.1 A ton as used in this practice is 907 kg (2000 lb).
1.2.2 Values in SI units shall be obtained by measurement in
SI units or by appropriate conversion, using the Rules for
Conversion and Rounding given in Standard IEEE/ASTM SI
10, of measurement made in other units.
1.3 This standard does not purport to address all of the
safety concerns, if any, associated with its use. It is the
responsibility of the user of this standard to establish appro
priate safety and health practices and determine the applica
bility of regulatory limitations prior to use.
2. Referenced Documents
2.1 ASTM Standards:
C 91 Speciﬁcation for Masonry Cement
2
C 109 Test Method for Compressive Strength of Hydraulic
Cement Mortars (Using 2in. or 50mm Cube Specimens)
2
C 114 Test Methods for Chemical Analysis of Hydraulic
Cement
2
C 115 Test Method for Fineness of Portland Cement by the
Turbidimeter
2
C 150 Speciﬁcation for Portland Cement
2
C 151 Test Method for Autoclave Expansion of Portland
Cement
2
C 157 Test Method for Length Change of Hardened
HydraulicCement Mortar and Concrete
3
C 185 Test Method for Air Content of Hydraulic Cement
Mortar
2
C 186 Test Method for Heat of Hydration of Hydraulic
Cement
2
C 191 Test Method for Time of Setting of Hydraulic Ce
ment by Vicat Needle
2
C 204 Test Method for Fineness of Hydraulic Cement by
Air Permeability Apparatus
2
C 227 Test Method for Potential Alkali Reactivity of
CementAggregate Combinations (MortarBar Method)
3
C 265 Test Method for Calcium Sulfate in Hydrated Port
land Cement Mortar
2
C 266 Test Method for Time of Setting of HydraulicCement
Paste by Gillmore Needles
2
C 451 Test Method for Early Stiffening of Hydraulic Ce
ment (Paste Method)
2
C 452 Test Method for Potential Expansion of Hydraulic
Cement Mortars Exposed to Sulfate
2
C 563 Test Method for Optimum S0
3
in Hydraulic Cement
Using 24 h Compressive Strength
2
C 595 Speciﬁcation for Blended Hydraulic Cements
2
C 845 Speciﬁcation for Expansive Hydraulic Cement
2
C 1012 Test Method for Length Change of Hydraulic
Cement Mortars Exposed to a Sulfate Solution
2
E 11 Speciﬁcation for WireCloth Sieves for Testing Pur
poses
4
IEEE/ASTM SI 10 Standard for Use of the International
System of Units (SI): The Modern Metric System
4
2.2 ACI Standard:
225.1R Guide to the Selection and Use of Hydraulic Ce
ments
5
3. Terminology
3.1 Deﬁnitions of Terms Speciﬁc to This Standard:
3.1.1 lot (of cement)—speciﬁc quantity of cement offered
for inspection at any one time. A lot may be one or more
storage bins ﬁlled consecutively. A lot may also be the contents
of one or more transport units representing cement drawn from
the same storage bin.
3.1.2 reduced testing rate—test program that provides for
the testing of only two samples from any given lot of samples
obtained and prepared for testing at the normal rate as
described herein. The program utilizes probability factors and
is so designed that when results from the two samples fulﬁll the
requirements of the program it may be said with 95 %
conﬁdence that less than 5 % of the samples would be outside
the speciﬁcation limits.
1
This practice is under the jurisdiction of ASTM Committee C1 on Cement, and
is the direct responsibility of Subcommittee C01.95 on Methods of Test.
Current edition approved Oct. 10, 1995. Published December 1995. Originally
published as C 183 – 44. Last previous edition C 183 – 95.
2
Annual Book of ASTM Standards, Vol 04.01.
3
Annual Book of ASTM Standards, Vol 04.02.
4
Annual Book of ASTM Standards, Vol 14.02.
5
Detailed requirements for this sieve are given in Speciﬁcation E 11.
1
Copyright © ASTM, 100 Barr Harbor Drive, West Conshohocken, PA 194282959, United States.
Để xem tài liệu đầy đủ. Xin vui lòng
Đăng nhập
Nếu xem trực tuyến bị lỗi, bạn có thể tải về máy để xem.
ASTM C183 : Sampling and the Amount of Testing of Hydraulic Cement

Người đăng:
kien098
5
Tài liệu rất hay!
Được đăng lên bởi
honhathoang0

1 giờ trước
Đúng là cái mình đang tìm. Rất hay và bổ ích. Cảm ơn bạn!
6
Vietnamese
ASTM C183 : Sampling and the Amount of Testing of Hydraulic Cement
9
10
228